**HAL Id: hal-00426291**

**https://hal.archives-ouvertes.fr/hal-00426291v3**

### Preprint submitted on 29 Dec 2010

**HAL** is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

### L’archive ouverte pluridisciplinaire **HAL, est** destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.

**Monte Carlo Study of the Spin Transport in Magnetic** **Materials**

### Yann Magnin, K. Akabli, Hung The Diep, Isao Harada

**To cite this version:**

### Yann Magnin, K. Akabli, Hung The Diep, Isao Harada. Monte Carlo Study of the Spin Transport in

### Magnetic Materials. 2009. �hal-00426291v3�

### Monte Carlo Study of the Spin Transport in Magnetic Materials

### Y. Magnin

^{a}

### , K. Akabli

^{a,b}

### , H. T. Diep

^{∗,a}

### , I. Harada

^{b}

a

*Laboratoire de Physique Th´* *eorique et Mod´* *elisation,* *CNRS UMR 8089, Universit´* *e de Cergy-Pontoise,*

*2, avenue Adolphe Chauvin, F-95302 Cergy-Pontoise Cedex, France.*

b

*Graduate School of Natural Science and Technology, Okayama University* *3-1-1 Tsushima-naka, Kita-ku, Okayama 700-8530, Japan..*

### Abstract

### The resistivity in magnetic materials has been theoretically shown to depend on the spin-spin correlation function which in turn depends on the magnetic-field, the density of conduction electron, the magnetic ordering stability, etc. However, these theories involved a lot of approximations, so their validity remained to be confirmed. The purpose of this work is to show by newly improved extensive Monte Carlo (MC) simulation the resistivity of the spin resistivity from low-T ordered phase to high-T paramagnetic phase in ferromagnetic and antiferromagnetic films. We take into account the interaction between the itinerant spins and the localized lattice spins as well as the interaction between itinerant spins themselves.

### We show that in ferromagnets the resistivity shows a sharp peak at the magnetic phase transition in agreement with previous theories in spite of their numerous approximations. Resistivity in antiferromagnets on the other hand shows no peak for the SC, BCC and diamond lattices. Discussion on the origin of these resistivity behaviors is given.

*Key words:* spin transport, Monte Carlo simulation, magnetic resistivity, magnetic materials *PACS:* 72.25.-b, 75.47.-m

### 1. Introduction

### The magnetic resistivity has been extensively studied by both theories and experiments in the last fifty years.

### Experiments have shown that the resistivity indeed de- pends on the itinerant spin orientation and the lattice spin ordering [1–6]. At low temperature (T ), the main magnetic scattering is due to spin-wave excitations [7, 8].

### The resistivity is proportional to T

^{2}

### . However at higher T the spin-wave theory is not valid, such a calculation of the resistivity is not possible, in particular in the critical region around the Curie temperature T

c### in simple ferro- magnets, let alone other complicated magnetic orderings.

### Experiments on various magnetic materials have found in particular an anomalous behavior of the resistivity at the critical temperature where the system undergoes the ferromagnetic-paramagnetic phase transition [2–6]. Very recent experiments such as those performed on ferromag- netic SrRuO

3### thin films[9], superconducting BaFe

2### As

2### sin- gle crystals[10], La

1−x### Sr

x### MnO

3### [11], Mn

1−x### Cr

x### Te[12] and other compounds[13–16] show different forms of anomaly of the magnetic resistivity at the transition temperature.

### de Gennes and Friedel’s first explanation in 1958[17] for the resistivity behavior near T

c### was based on the inter- action between the spins of conduction electrons and the lattice spins. The resistivity was thus expected to depend

∗

### To whom correspondence should be addressed.

*Email address:* diep@u-cergy.fr (H. T. Diep )

### strongly on the spin ordering of the system. They have suggested that the magnetic resistivity is proportional to the spin-spin correlation, therefore it should behave as the magnetic susceptibility with a divergence at T

c### due to ”long-range” fluctuations of the magnetization. Other authors [18–20] subsequently suggested that the shape of the resistivity results mainly from ”short-range” correla- tion at T ≥ T

c### . Fisher and Langer [19] have shown in particular that the form of the resistivity cusp depends on the correlation range. To see more details on the role of the spin-spin correlation, we quote a work by Haas[21] and a more recent work of Kataoka[22] where the spin-spin corre- lation function has been calculated. Recently, Zarand et al [23] have used the picture that the itinerant spin is mainly scattered by impurities which are characterized by a ”lo- calization length” in the sense of Anderson’s localization.

### They found that the peak’s height depends on this localiza-

### tion length. Note that since the giant magnetoresistance

### (GMR) was discovered experimentally twenty years ago in

### magnetic multilayers [24, 25], intensive investigations on

### the spin resistivity, both experimentally and theoretically,

### have been carried out[26, 27]. The ”spintronics” was born

### with a spectacular rapid development in relation with in-

### dustrial applications. For recent overviews, the reader is

### referred to Refs. [28] and [29]. In spite of these inten-

### sive investigations, except our works[30, 31], there have

### been no Monte Carlo (MC) simulations performed regard-

### ing the temperature dependence of the spin transport. In

### these works , we have investigated by MC simulations the

### effects of magnetic ordering on the spin current in mag- netic multilayers.

### In this paper we improve our previous MC simulations to study the transport of itinerant electrons in ferromag- netic and antiferromagnetic crystals. We use the Ising model and take into account interactions between lattice spins and itinerant spins. We show that in ferromagnets we obtain, with our new MC averaging method, much bet- ter results for the magnetic resistivity which shows a huge peak at the transition temperature while in antiferromag- nets, the resistivity does not show such a peak.

### The paper is organized as follows. Section 2 is de- voted to the description of our model and the rules that govern its dynamics. In section 3, we describe our MC method and discuss the results we obtained for ferromag- nets. Results on antiferromagnets are shown in Section 4.

### Concluding remarks are given in Section 5.

### 2. Model

*2.1. Interactions*

### We consider a thin film of FCC structure with two symmetrical (001) surfaces. The total number of cells is N

x### × N

y### × N

z### where each cell has four spins. Spins lo- calized at FCC lattice sites are called ”lattice spins” here- after. They interact with each other through the following Hamiltonian

### H

^{l}

### = − J X

hi,ji

### S

i### · S

j### , (1)

### where S

i### is the Ising spin at lattice site i, P

hi,ji

### indi- cates the sum over every nearest-neighbor (NN) spin pair (S

i### , S

j### ), J being the NN interaction. We consider in this paper both J > 0 (ferromagnets) and J < 0 (antiferro- magnets).

### We consider a flow of itinerant spins interacting with each other and with the lattice spins. The interaction be- tween itinerant spins is defined by

### H

m### = − X

hi,ji

### K

i,j### s

_{i}

### · s

_{j}

### , (2)

### where s

i### is the itinerant Ising spin at position ~r

i### , and P

hi,ji

### denotes a sum over every spin pair ( s

_{i}

### , s

_{j}

### ). The interaction K

i,j### depends on the distance between the two spins, i.e.

### r

ij### = | r

i### − r

j### | . A specific form of K

i,j### will be chosen below.

### The interaction between itinerant spins and lattice spins is given by

### H

^{r}

### = − X

hi,ji

### I

i,j### s

i### · S

j### , (3)

### where the interaction I

i,j### depends on the distance between the itinerant spin s

_{i}

### and the lattice spin S

_{i}

### . For the sake

### of simplicity, we assume the same form for K

i,j### and I

i,j### , namely,

### K

i,j### = K

0### exp( − r

ij### ) (4) I

i,j### = I

0### exp( − r

ij### ) (5) where K

0### and I

0### are constants.

*2.2. Monte Carlo Method*

### Before calculating the resistivity, we determine the crit- ical temperature T

c### below which the system is in the or- dered phase using Eq. (1). To this end, we perform standard Metropolis MC simulations to determine various physical quantities at different T [32].

### Once the lattice is equilibrated at a given T, we inject N

0### itinerant spins into the system. The itinerant spins move in the x direction under the effect of an electric field.

### We use the periodic boundary conditions to ensure that the average density of itinerant spins remains constant with evolving time (stationary regime).

### Note that unlike in the previous works[30, 31] where the lattice spin configuration is frozen while calculating the resistivity, we use here several thousands of configura- tions in each of which the resistivity is averaged with many thousands of passages. In our previous works, though the overall number of MC steps per spin was as high as in this work, the fact that we have used only a dozen lattice configurations for resistivity calculation has shown strong fluctuations in the result. In this work, we have made a new device in two steps:

### i) For each lattice configuration all itinerant spins move through the system during typically one thousand MC steps. Then we thermalize again the lattice for several thousands of MC steps before continuing the averaging of the resistivity for another thousand MC steps per spin. We repeat this cycle for 200 times. In doing so, each itinerant spin was averaged over 10

^{6}

### MC step using ”uncorrelated”

### 200 lattice configurations in all.

### ii) The resistivity R is defined as R =

^{1}

_{n}

### where n is the number of itinerant spins crossing a unit area perpen- dicular to the x direction per unit of MC time. To know this number, we count them at three ”detector” surfaces perpendicular to the x direction: the first at N

x### /4, the second at N

x### /2 and the third at 3N

x### /4. Averaging the re- sistivity at these three system positions helps to improve further the results (in our previous works[31] we counted them only at the end of the sample).

### As will be shown below, these extensive configuration and space averages give much better results with respect to those in previous works. The dynamics of itinerant spins is governed by the following interactions:

### i) an electric field E which is applied in the x direction.

### Its energy is given by

### H

^{E}

### = − eE · r

i### , (6) where r

i### is the distance traveled by the itinerant spin s

i### in a MC step, e its charge. The orientation of r

i### is taken

### 2

### at random, its magnitude is taken from a uniform distri- bution between 0 and r

0### where r

0### is the nearest-neighbor distance;

### ii) a chemical potential term (”concentration gradient”

### effect) given by

### H

^{c}

### = Dn(r), (7)

### where n(r) is the concentration of itinerant spins in a sphere of radius D

2### centered at r. D is a constant taken equal to K

0### for simplicity;

### iii) interactions between a given itinerant spin and lat- tice spins inside a sphere of radius D

1### (Eq. 3);

### iv) interactions between a given itinerant spin and other itinerant spins inside a sphere of radius D

2### (Eq. 2).

### The simulation is carried out as follows: at a given T we calculate the energy of an itinerant spin s

_{i}

### by taking into account all the interactions described above. Then we tentatively move the spin under consideration to a new position with a step r

_{i}

### in an arbitrary direction. Note that this move is immediately rejected if the new position is in- side a sphere of radius ∆

0### centered at a lattice spin or an itinerant spin. This excluded space represents the Pauli exclusion principle in the one hand, and the interaction with lattice phonons on the other hand. If the new posi- tion does not lie in a forbidden region of space, then the move is accepted with a probability given by the standard Metropolis algorithm[32].

### 3. Results on Ferromagnetic Thin Films

### We let N

0### itinerant spins travel through the system sev- eral thousands of passages until a steady state is reached before averaging the spin resistivity.

### The parameters we use in our calculations for ferro- magnets are s = S = 1 and N

x### = N

y### = 20 and N

z### = 8.

### Other parameters are D

1### = D

2### = 1 (all distances are in unit of the FCC cell length), K

0### = I

0### = 0.5 and D = 0.5 unless otherwise stated, N

0### = 8 × 20

^{2}

### (namely one itiner- ant spin per FCC unit cell), ∆

0### = 0.05 and r

0### = √

### 2/2, the FCC nearest-neighbor distance. At each T the equilibra- tion time for the lattice spins lies around 10

^{6}

### MC steps per spin and we compute statistical averages for the resistiv- ity over 10

^{6}

### MC steps per spin. Note that, as described in subsection 2.2, in this work the averaging length 10

^{6}

### MC steps per spin has been divided into 200 segments of 5000 MC steps; between two consecutive segments we thermal- ize again our lattice over several thousands of MC steps par spin to explore a maximum of lattice configurations encountered by itinerant spins. In doing so we reduce sta- tistical fluctuations observed in our old works[30, 31].

### We show in Fig. 1 the lattice magnetization versus T for N

z### = 8, N

x### = N

y### = 20, J = 1. We find T

c### ≃ 9.58 for the critical temperature of the lattice spins.

### We show in Fig. 2 the resistivity versus T without magnetic field for several values of I

0### , interaction between itinerant spins and lattice spins. Several remarks are in order:

### Figure 1: Lattice magnetization versus temperature T for N

_{z}

### = 8, N

_{x}

### = N

_{y}

### = 20. T

_{c}

### is ≃ 9 . 58 in unit of J = 1.

### Figure 2: Resistivity R in arbitrary unit versus temperature T for several values of I

_{0}

### : 2 (black circles), 1 (void circles), 0.5 (black triangles). Other parameters: N

x

### = N

y

### = 20, N

z

### =8, E = 1, K

_{0}

### = 0 . 5, D = 0 . 5, D

_{1}

### = 1.

### i) As seen here, no significant fluctuations of the data are observed in the whole temperature range, thanks to our new averaging device (see subsection 2.2).

### ii) At T

c### , R exhibits a peak at the transition temper- ature. The height of the peak decreases with decreasing I

0### . We see thus that the peak is a consequence of the in- teraction between itinerant spins and lattice spins. The resistivity shows almost no peak for I

0### = 0.5. This case corresponds to a metal where the interaction between itin- erant and lattice spins is very weak.

### iii) We can explain the existence of the peak by the fol- lowing argument: the peak is due to the coupling through I

0### of itinerant spins to the fluctuations of the lattice spins in the critical region around T

c### . In our recent work, we found from our MC simulation[31] that the resistivity’s peak is due to the scattering by antiparallel-spin clusters which exist when one enters the critical region. Below the transition temperature, there exists a single large cluster of lattice spins with some isolated ”defects” (i. e. clusters of antiparallel spins), so that the resistance decreases with decreasing T just after T

c### .

### iv) However, at very low T , the resistivity increases

### with decreasing T . The origin of this behavior comes from

### the freezing of the itinerant spins due to their interaction

### with lattice spins and with themselves. This is very similar

### to the crystallization of interacting particles at low T . We

### have tested this interpretation by reducing the strength of

### the interactions K

0### and I

0### . As a matter of fact, R increases

### more slowly with decreasing T . This is seen in Fig. 2 at low

### Figure 3: Travel path of an itinerant spin at T = 5 (upper) and at T = 9 . 79 (lower) for I

_{0}

### = 2. Other parameters are the same as in Fig. 2. See text for comments.

### T where R is smaller for smaller I

0### . Note that the increase of R at very low T was observed in many experiments on various materials not limited to ferromagnets[10–12, 14].

### v) In the paramagnetic phase, as T increases, small clusters will be broken more and more into single disor- dered spins, so that there is no more energy barrier be- tween successive positions of itinerant spins on their tra- jectory. The resistance, though high, is thus decreasing with increasing T and saturated as T → ∞ .

### During the simulation, we have followed one itinerant spin among 3200 and recorded its successive positions. We show in Fig. 3 its travel path at T = 5 where R is very low and at T = 9.79 where R is highest. As seen, even at T = 5, the spin spends a lot of time to overcome the scattering by lattice spins. Almost four thousands of trial moves are needed to get through the system. Meanwhile, at T = 9.79, the spin under consideration spends all this time in a small area. Note that at this peak’s temperature, very few spins can go until the end unless we increase the electric field.

*3.1. Effect of magnetic field.*

### Kataoka[22] has shown by a Boltzmann’s equation for- malism that the magnetic field reduces the peak’s height.

### This is what we observed in simulations. We show re- sults of R for several fields in Fig. 4. The peak reduction is stronger for stronger fields. This is easily understood:

### when a magnetic field is applied on a ferromagnet, the phase transition is suppressed because the magnetization is not zero at any T . The field reduces critical fluctuations, and hence the number of clusters of antiparallel spins. The peak of the resistivity is therefore reduced and disappears at high fields.

### To close this section, let us emphasize that in ferromag- nets, we have improved the previous results[31] by using a new averaging procedure. We found that the height of the peak is intimately related to the strength of the interaction between itinerant spins and lattice spins (Fig. 2).

### Figure 4: Resistivity R in arbitrary unit versus temperature T , for different magnetic fields B : 0 (black circles), 0.25 (void circles), 0.5 (black triangles), 0.75 (void triangles). I

_{0}

### = 2 and other parameters taken the same as in Fig. 2.

### 4. Results on Antiferromagnetic Thin Films In the case of antiferromagnets, we study first a film with simple cubic (SC) lattice structure. This is because the FCC lattice used in the ferromagnetic case shown above becomes fully frustrated if we use an antiferromagnetic in- teraction. The frustrated case is very particular [33], it cannot be treated on the same footing as the non frus- trated case.

### Before showing the results on a SC antiferromagnet, let us emphasize the following point. The picture of de- fect clusters of down spins embedded in a up-spin sea that we used above to explain the behavior of the resistivity in ferromagnets should be modified in the case of antifer- romagnets: in antiferromagnets defects are domain walls, clusters on the two sides of a wall both have antiferro- magnetic ordering with opposite parity. An itinerant spin crossing a domain wall does not have the same scattering as in a ferromagnet. Its scattering depends on the num- bers of up spins and down spins in the sphere of radius D

1### . In other words, the scattering depends on the energy land- scape in the crystal: the itinerant spin will stay a longer time where its energy is low, and a shorter time where its energy is high.

### The resistivity versus T in zero magnetic field is shown in Fig. 5 with D

1### = D

2### = 1. Several remarks are in order: i) one observes the absence of a peak of R; ii) the variation of R with T has the same shape as the internal energy versus T shown in Fig. 6, therefore dR/dT shows a peak similar to the specific heat. The peak of dR/dT has been experimentally observed in many materials, in particular in MnSi [3, 4] among others [2].

### The absence of a peak at T

N### observed here certainly comes from the fact that the motion of an itinerant elec- tron is not sharply slowed down at T

N### by numerous clus- ters of opposite spins. Let us say it again in another man- ner: the absence of a peak at the transition is due to the fact that the motion of an itinerant spin depends on its immediate environment: in ferromagnets, the variation of its energy ∆E going from a ”parallel” cluster to a nearby

### ”defect” (or antiparallel) cluster is much larger than the

### energy variation going from a cluster of antiferromagnetic

### 4

### Figure 5: SC AF case. Resistivity R in arbitrary unit versus temperature T , in zero magnetic field, with electric field E = 1, I

_{0}

### = K

_{0}

### = 0 . 5.

### Figure 6: SC AF case. Internal energy E in unit | J | = 1 versus temperature T , in zero magnetic field, with electric field E = 1, I

_{0}

### = K

_{0}

### = 0 . 5.

### ordering to a cluster which is a defect but a defect with an antiferromagnetic structure in the SC antiferromagnetic case. The smaller ∆E gives rise to a larger spin mobility i. e. a smaller R. Note that experimental data show just a shoulder in antiferromagnetic LaFeAsO[16].

### We show now in Fig. 7 the effect of D

1### on the resistiv- ity at a given temperature. We observe here an oscillatory behavior of R. By analyzing the ratio of numbers of up spins and down spins in the sphere of radius D

1### , we found that this ratio oscillates with varying D

1### : the maxima (minima) of R correspond to the largest (smallest) num- bers of parallel (antiparallel) spins in the sphere. This finding is consistent with what we said before, namely R is large when the energy of itinerant spin is low (i. e. large number of parallel spins).

### We show in Fig. 8 the resistivity versus T for several D

1### . As seen here, the change of R at a given T > T

N### with varying D

1### is much smaller than that for T < T

N### . It is interesting to note that R does not depend on D

1### at T

N### . Further analysis should be carried out to understand this behavior at the transition point.

### Finally, to compare with the SC AF case, let us show the results of the BCC and diamond-lattice antiferromag- nets in Figs. 9 and 10. As seen, these cases shows no peak for any value of D

1### . Note that R in both cases increases as T decreases to zero, unlike the SC AF case. The origin of this increase lies in the freezing of itinerant spins at low T . The degree of freezing depends on the lattice structure and on the strength of the interactions of the itinerant spins

### Figure 7: SC AF case. Resistivity R in arbitrary unit versus D

1### at T = 1, in zero magnetic field, with electric field E = 1, I

_{0}

### = K

_{0}

### = 0 . 5.

### Figure 8: SC AF case. Resistivity R versus T for several values of D

_{1}

### : 1 (black circles), 1.2 (void triangles), 1.4 (black triangles), 1.6 (void circles), E = 1, B = 0, I

_{0}

### = K

_{0}

### = 0 . 5, D = 0 . 35.

### with their environment as discussed in the ferromagnetic section.

*4.1. Discussion*

### In the case of ferromagnets, the coupling of the motion of itinerant spins to the correlation of the lattice spins gives rise to the peak of the resistivity in the transition region.

### Depending on the strength of this coupling, the peak can be very sharp or rounded at T

c### . The picture of scattering by clusters suggested by us is naturally consistent with the correlation interpretation.

### In the case of antiferromagnets, the polarized itinerant spins are coupled to both parallel and antiparallel lattice spins. Due to the opposite correlation signs, their respec-

### Figure 9: BCC AF case. Resistivity R versus T for several values of

### D

_{1}

### : 1 (black circles), 1.2 (void triangles), 1.4 (black triangles), 1.6

### (void circles), E = 1, B = 0, I

_{0}

### = K

_{0}

### = 1, D = 0 . 5.

### Figure 10: Diamond-lattice AF case. Resistivity R versus T for D

1### : 0.5 (black triangles), 0.75 (black circles), 1 (void circles). E = 1, B = 0, I

_{0}

### = K

_{0}